J. Phys. Chem. B 2006, 110, 25521-25524
Electronic Properties of Doped Molecular Thin Films Measured by Kelvin Probe Force Microscopy† O. Tal and Y. Rosenwaks* School of Electrical Engineering, Tel AViV UniVersity, Tel AViV 69978, Israel ReceiVed: August 14, 2006; In Final Form: September 28, 2006
We report on high-resolution electronic measurements of doped organic thin-film transistors using Kelvin probe force microscopy. Measurements conducted on field effect transistors made of N,NI-diphenyl-N,NIbis(1-naphthyl)-1,1I-biphenyl-4,4I-diamine p-doped with tetrafluoro-tetracyanoquinodimethane have allowed us to determine the rich structure of the doping-induced density of states. In addition, the doping process changes only slightly the Fermi energy position with respect to the highest occupied molecular orbital level center. The moderate change is explained by two counter-acting effects on the Fermi energy position: the doping-induced additional charge and the broadening of the density of states.
I. Introduction The field of semiconducting organic molecular films is developing very fast, driven by the enormous potential demonstrated by these materials for applications in optoelectronics and inexpensive electronics such as light-emitting diodes, field effect transistors, and photovoltaic cells. As an example, organic thin-film transistors (OTFTs) present several possible advantages, such as low-cost processing, mechanical flexibility, and patterning for large-area applications. Improving the performance of OTFTs requires a deep understanding of charge carrier transport mechanisms through the organic layer. Although material technology advanced significantly over the last two decades, a fundamental understanding of the basic electronic and optical processes in these materials is still rather poor, and extensive research is necessary. A good example of the above is the insertion of electronically active dopant molecules (i.e., electron donors or acceptors) into organic thin films, which has already been demonstrated by several groups. Dopants are introduced either intentionally to improve the film conductivity,1 modify charge injection barriers,2 add functionality (e.g., a pn junction3), and modify the film optical properties4 or unintentionally as synthesis impurities5, solution residuals,6 and chemically induced doping,7 which deteriorate the performance of the organic material. In any case, an accurate understanding of the density of states (DOS) energy distribution and how it is affected by molecular doping is one of the keys to advancing basic research on and technological applications of organic semiconductor films, since most electronic properties of organic semiconductors are closely related to the shape of the DOS8,9 In this work, we use high lateral resolution Kelvin probe force microscopy (KPFM) to measure several electronic properties of doped organic molecular thin films. KPFM has already been utilized for the study of charge mobility in OTFTs,10 and the potential drops at the source and drain contacts of operating OTFTs.11,12 Here, it is demonstrated that by using KPFM measurements across OTFT with a relatively thin organic film †
Part of the special issue “Arthur J. Nozik Festschrift”. * Author to whom correspondence should be addressed. E-mail: [email protected]
(10 nm) it is possible to measure quantitatively the energy distribution of the hole DOS and the Fermi level position. II. Experimental Section A typical OTFT structure used in all measurements is schematically shown in Figure 1. The OTFT substrates (fabricated by the Tessler group at the TechnionsIsrael Institute of Technology) consisted of a heavily doped p-type silicon gate electrode, a thermally grown 90 nm silicon oxide gate insulator, and 50-nm-thick gold strips evaporated on the oxide to form source and drain electrodes separated by 16 µm. A thin film (10 nm) of N,NI-diphenyl-N,NI-bis(1-naphthyl)-1,1I-biphenyl4,4I-diamine (a-NPD) was deposited on the substrate by sublimation in an ultrahigh vacuum chamber. Doped a-NPD films were formed by coevaporation of tetrafluoro-tetracyanoquinodimethane (F4TCNQ) with the host molecules (by the Kahn group at Princeton University). The OTFTs were transported under nitrogen atmosphere to a glovebox ( 0. In the case of nonnegligible level bending (Figure 3b), the measured VL(x) is smaller because part of the applied gate voltage induces band bending in the organic layer. Our method for DOS measurement is feasible when the energy level bending perpendicular to the gate can be neglected. According to our numerical calculations18 conducted for a 10nm-thick organic layer in an OFET structure and different Gaussian DOS distributions, the induced charge is homogeneously distributed across the organic film width, and the energy level bending from the film surface to the film/gate insulator interface is negligible up to a certain VGS value. Above this given VGS value,19 the conducting channel is squeezed toward the gate insulator, and the level bending is not negligible; this behavior has already been reported elsewhere.20,21 Under negligible level bending conditions, the shift of the energy levels (VL) for different VGS values with respect to the level position at VGS ) Vt can be measured directly by KPFM based on eq 1. The hole concentration at any lateral location x in the channel is given by
p(x) ) -
COX (V - Vt - VL(x)) qdorg GS
where COX is the silicon oxide (insulating layer) capacitance per unit area and dorg is the organic film thickness. Equation 2 is only valid when the charge concentration is homogeneously distributed across the organic film depth. However, the hole concentration in the channel is given by
∫-∞∞ g(E)(1 - fFD(E)) dE
where g(E) is the DOS relevant for holes and fFD(E) is the Fermi-Dirac distribution. With the hole concentration and the energy level shift, the hole DOS is calculated as described in
Electronic Properties of Doped Thin Films
J. Phys. Chem. B, Vol. 110, No. 50, 2006 25523
Figure 4. Topography curve (bottom) and VL curves (top) measured by KPFM across the transistor top surface for VDS ) 0 V and -16.5 V e VGS e 0 V.
Figure 5. DOS vs energy relative to Etf (Ef at VGS ) Vt) for undoped (solid triangles) and doped (solid circles) samples. The solid curves are fittings of a Gaussian function (eq 2, curve A) and an exponential function (eq 4, curve B) to given ranges in the undoped sample DOS curve and a fitting of eq 3 (curve C) to the doped sample DOS curve.
Appendix A to give
This analytic expresion, which has no fitting parameters, is used to obtain the DOS from the measured VL. Figure 4 shows VL (solid curves) and topography (dashed curve) profiles measured simultaneously across an undoped transistor. The protruding regions on the left and right sides of the bottom topography profile correspond to the source and drain contacts, while the conduction channel is located between them (see Figure 1 for comparison). The potential of the grounded source and drain appears as the flat portion at each end of the VL curves, and the potential distribution across the organic channel is seen between them. The VL curves were measured for VGS values ranging from 0 to -16.5 V across relatively smooth regions of the organic layer (roughness,